#------------------------------------------------------------------------------
#$Date: 2016-03-23 16:17:38 +0200 (Wed, 23 Mar 2016) $
#$Revision: 179370 $
#$URL: svn://www.crystallography.net/cod/cif/4/32/67/4326715.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_4326715
loop_
_publ_author_name
'Qisheng Lin'
'John D. Corbett'
_publ_contact_author_address
;Dept. of Chem.
Iowa State University
Ames, IA, 50011
;
_publ_contact_author_email       jcorbett@iastate.edu
_publ_contact_author_name        'John D. Corbett'
_publ_section_title
;
 Exploratory Syntheses and Structures of SrAu4.3In1.7 and CaAg3.5In1.9:
 Electron-Poor Intermetallics with Diversified Polyanionic Frameworks That
 Are Derived from the CaAu4In2 Approximant
;
_journal_name_full               'Inorganic Chemistry'
_journal_page_first              11091
_journal_page_last               11098
_journal_paper_doi               10.1021/ic2016275
_journal_volume                  50
_journal_year                    2011
_chemical_formula_sum            'Ca25.82 Cd140.99'
_chemical_formula_weight         16862.23
_chemical_name_systematic
; 
 ? 
;
_space_group_IT_number           191
_symmetry_cell_setting           hexagonal
_symmetry_space_group_name_Hall  '-P 6 2'
_symmetry_space_group_name_H-M   'P 6/m m m'
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                120.00
_cell_formula_units_Z            1
_cell_length_a                   20.660(3)
_cell_length_b                   20.660(3)
_cell_length_c                   9.4100(19)
_cell_measurement_reflns_used    1713
_cell_measurement_temperature    293(2)
_cell_measurement_theta_max      28.29
_cell_measurement_theta_min      1.14
_cell_volume                     3478.4(10)
_computing_cell_refinement       'Bruker XSCANS'
_computing_data_collection       'Bruker XSCANS'
_computing_data_reduction        'Bruker SHELXTL'
_computing_molecular_graphics    'Bruker SHELXTL'
_computing_publication_material  'Bruker SHELXTL'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      293(2)
_diffrn_measured_fraction_theta_full 0.992
_diffrn_measured_fraction_theta_max 0.992
_diffrn_measurement_device_type  'Smart CCD'
_diffrn_measurement_method       'ω scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0414
_diffrn_reflns_av_sigmaI/netI    0.0142
_diffrn_reflns_limit_h_max       27
_diffrn_reflns_limit_h_min       -26
_diffrn_reflns_limit_k_max       15
_diffrn_reflns_limit_k_min       -27
_diffrn_reflns_limit_l_max       12
_diffrn_reflns_limit_l_min       -12
_diffrn_reflns_number            22038
_diffrn_reflns_theta_full        28.29
_diffrn_reflns_theta_max         28.29
_diffrn_reflns_theta_min         1.14
_exptl_absorpt_coefficient_mu    21.928
_exptl_absorpt_correction_T_max  0.789
_exptl_absorpt_correction_T_min  0.434
_exptl_absorpt_correction_type   empirical
_exptl_absorpt_process_details   SADABS
_exptl_crystal_colour            silver
_exptl_crystal_density_diffrn    8.050
_exptl_crystal_description       irregular
_exptl_crystal_F_000             7275
_exptl_crystal_size_max          0.038
_exptl_crystal_size_mid          0.025
_exptl_crystal_size_min          0.011
_refine_diff_density_max         8.637
_refine_diff_density_min         -4.549
_refine_diff_density_rms         0.355
_refine_ls_extinction_coef       0.000275(15)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_extinction_method     SHELXL
_refine_ls_goodness_of_fit_ref   1.147
_refine_ls_matrix_type           full
_refine_ls_number_parameters     98
_refine_ls_number_reflns         1713
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.147
_refine_ls_R_factor_all          0.0386
_refine_ls_R_factor_gt           0.0375
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0175P)²+151.3610P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0775
_refine_ls_wR_factor_ref         0.0787
_reflns_number_gt                1671
_reflns_number_total             1713
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            ic2016275_si_002_2.cif
_cod_data_source_block           CaAg3.5In1.9
_cod_database_code               4326715
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-y, x-y, z'
'-x+y, -x, z'
'-x, -y, z'
'y, -x+y, z'
'x-y, x, z'
'y, x, -z'
'x-y, -y, -z'
'-x, -x+y, -z'
'-y, -x, -z'
'-x+y, y, -z'
'x, x-y, -z'
'-x, -y, -z'
'y, -x+y, -z'
'x-y, x, -z'
'x, y, -z'
'-y, x-y, -z'
'-x+y, -x, -z'
'-y, -x, z'
'-x+y, y, z'
'x, x-y, z'
'y, x, z'
'x-y, -y, z'
'-x, -x+y, z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
Cd1 Cd 0.13541(4) 0.27083(7) 0.0000 0.0169(3) Uani 1 4 d S
Cd2 Cd 0.13175(5) 0.40814(5) 0.0000 0.0160(2) Uani 1 2 d S
Cd3 Cd 0.26081(3) 0.52162(5) 0.15576(10) 0.0179(2) Uani 1 2 d S
Cd4 Cd 0.41499(7) 0.0000 0.0000 0.0221(3) Uani 1 4 d S
Cd5 Cd 0.18034(3) 0.36067(5) 0.25149(10) 0.0182(2) Uani 1 2 d S
Cd6 Cd 0.13642(8) 0.0000 0.0000 0.0323(4) Uani 1 4 d S
Cd7 Cd 0.61615(3) 0.23229(6) 0.33377(11) 0.0227(2) Uani 1 2 d S
Cd8 Cd 0.3333 0.6667 0.0000 0.0236(5) Uani 1 12 d S
Cd9 Cd 0.10945(4) 0.45452(4) 0.27470(8) 0.02414(18) Uani 1 1 d .
Cd10 Cd 0.38840(8) 0.0000 0.5000 0.0250(3) Uani 1 4 d S
Cd11 Cd 0.55025(5) 0.10050(9) 0.5000 0.0254(3) Uani 1 4 d S
Cd12 Cd 0.5000 0.0000 0.24968(15) 0.0212(3) Uani 1 4 d S
Cd13 Cd 0.08760(7) 0.31556(9) 0.5000 0.0423(4) Uani 1 2 d S
Cd14 Cd 0.09346(5) 0.18693(10) 0.26020(13) 0.0451(4) Uani 1 2 d S
Cd15 Cd 0.15226(12) 0.0000 0.5000 0.0416(5) Uani 1 4 d S
Cd16 Cd 0.0000 0.0000 0.0000 0.025 Uiso 0.306(11) 24 d SP
Cd17 Cd 0.0000 0.0000 0.0914(11) 0.025 Uiso 0.257(8) 12 d SP
Ca1 Ca 0.57496(10) 0.1499(2) 0.0000 0.0195(7) Uani 1 4 d S
Ca2 Ca 0.27593(14) 0.0000 0.2028(3) 0.0211(5) Uani 1 2 d S
Ca3 Ca 0.23930(11) 0.4786(2) 0.5000 0.0255(8) Uani 1 4 d S
Ca4 Ca 0.0000 0.0000 0.278(3) 0.084(8) Uani 0.90(4) 12 d SP
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Ca Ca 0.2262 0.3064 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Cd Cd -0.8075 1.2024 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
Cd6 Cd1 Cd6 60.74(6) 15 2
Cd6 Cd1 Cd5 119.00(2) 15 .
Cd6 Cd1 Cd5 119.00(2) 2 .
Cd6 Cd1 Cd5 119.00(2) 15 16
Cd6 Cd1 Cd5 119.00(2) 2 16
Cd5 Cd1 Cd5 111.63(6) . 16
Cd6 Cd1 Cd14 63.20(4) 15 16
Cd6 Cd1 Cd14 63.20(4) 2 16
Cd5 Cd1 Cd14 177.32(6) . 16
Cd5 Cd1 Cd14 65.70(4) 16 16
Cd6 Cd1 Cd14 63.20(4) 15 .
Cd6 Cd1 Cd14 63.20(4) 2 .
Cd5 Cd1 Cd14 65.70(4) . .
Cd5 Cd1 Cd14 177.32(6) 16 .
Cd14 Cd1 Cd14 116.98(8) 16 .
Cd6 Cd1 Cd2 118.32(3) 15 20
Cd6 Cd1 Cd2 179.07(4) 2 20
Cd5 Cd1 Cd2 61.31(3) . 20
Cd5 Cd1 Cd2 61.31(3) 16 20
Cd14 Cd1 Cd2 116.52(3) 16 20
Cd14 Cd1 Cd2 116.52(3) . 20
Cd6 Cd1 Cd2 179.07(4) 15 .
Cd6 Cd1 Cd2 118.32(3) 2 .
Cd5 Cd1 Cd2 61.31(3) . .
Cd5 Cd1 Cd2 61.31(3) 16 .
Cd14 Cd1 Cd2 116.52(3) 16 .
Cd14 Cd1 Cd2 116.52(3) . .
Cd2 Cd1 Cd2 62.61(5) 20 .
Cd6 Cd1 Ca2 66.61(4) 15 6
Cd6 Cd1 Ca2 116.29(6) 2 6
Cd5 Cd1 Ca2 61.64(3) . 6
Cd5 Cd1 Ca2 116.43(5) 16 6
Cd14 Cd1 Ca2 119.22(4) 16 6
Cd14 Cd1 Ca2 62.59(5) . 6
Cd2 Cd1 Ca2 62.98(5) 20 6
Cd2 Cd1 Ca2 114.13(5) . 6
Cd6 Cd1 Ca2 66.61(4) 15 15
Cd6 Cd1 Ca2 116.29(6) 2 15
Cd5 Cd1 Ca2 116.43(5) . 15
Cd5 Cd1 Ca2 61.64(3) 16 15
Cd14 Cd1 Ca2 62.59(5) 16 15
Cd14 Cd1 Ca2 119.22(4) . 15
Cd2 Cd1 Ca2 62.98(5) 20 15
Cd2 Cd1 Ca2 114.13(5) . 15
Ca2 Cd1 Ca2 67.59(8) 6 15
Cd6 Cd1 Ca2 116.29(6) 15 17
Cd6 Cd1 Ca2 66.61(4) 2 17
Cd5 Cd1 Ca2 116.43(5) . 17
Cd5 Cd1 Ca2 61.64(3) 16 17
Cd14 Cd1 Ca2 62.59(5) 16 17
Cd14 Cd1 Ca2 119.22(4) . 17
Cd2 Cd1 Ca2 114.13(5) 20 17
Cd2 Cd1 Ca2 62.98(5) . 17
Ca2 Cd1 Ca2 176.95(9) 6 17
Ca2 Cd1 Ca2 112.32(8) 15 17
Cd6 Cd1 Ca2 116.29(6) 15 2
Cd6 Cd1 Ca2 66.61(4) 2 2
Cd5 Cd1 Ca2 61.64(3) . 2
Cd5 Cd1 Ca2 116.43(5) 16 2
Cd14 Cd1 Ca2 119.22(4) 16 2
Cd14 Cd1 Ca2 62.59(5) . 2
Cd2 Cd1 Ca2 114.13(5) 20 2
Cd2 Cd1 Ca2 62.98(5) . 2
Ca2 Cd1 Ca2 112.32(8) 6 2
Ca2 Cd1 Ca2 176.95(9) 15 2
Ca2 Cd1 Ca2 67.59(8) 17 2
Cd4 Cd2 Cd9 70.15(2) 2 .
Cd4 Cd2 Cd9 70.15(2) 2 16
Cd9 Cd2 Cd9 128.25(5) . 16
Cd4 Cd2 Cd1 123.82(4) 2 .
Cd9 Cd2 Cd1 114.63(2) . .
Cd9 Cd2 Cd1 114.63(2) 16 .
Cd4 Cd2 Cd3 118.78(4) 2 .
Cd9 Cd2 Cd3 60.94(2) . .
Cd9 Cd2 Cd3 114.76(4) 16 .
Cd1 Cd2 Cd3 109.19(3) . .
Cd4 Cd2 Cd3 118.78(4) 2 16
Cd9 Cd2 Cd3 114.76(4) . 16
Cd9 Cd2 Cd3 60.94(2) 16 16
Cd1 Cd2 Cd3 109.19(3) . 16
Cd3 Cd2 Cd3 60.35(4) . 16
Cd4 Cd2 Cd5 121.54(2) 2 .
Cd9 Cd2 Cd5 61.51(2) . .
Cd9 Cd2 Cd5 168.24(4) 16 .
Cd1 Cd2 Cd5 59.10(2) . .
Cd3 Cd2 Cd5 62.21(3) . .
Cd3 Cd2 Cd5 110.31(3) 16 .
Cd4 Cd2 Cd5 121.54(2) 2 16
Cd9 Cd2 Cd5 168.24(4) . 16
Cd9 Cd2 Cd5 61.51(2) 16 16
Cd1 Cd2 Cd5 59.10(2) . 16
Cd3 Cd2 Cd5 110.31(3) . 16
Cd3 Cd2 Cd5 62.21(3) 16 16
Cd5 Cd2 Cd5 108.02(4) . 16
Cd4 Cd2 Cd2 177.49(3) 2 20
Cd9 Cd2 Cd2 109.10(2) . 20
Cd9 Cd2 Cd2 109.10(2) 16 20
Cd1 Cd2 Cd2 58.69(2) . 20
Cd3 Cd2 Cd2 59.176(19) . 20
Cd3 Cd2 Cd2 59.176(19) 16 20
Cd5 Cd2 Cd2 59.279(19) . 20
Cd5 Cd2 Cd2 59.279(19) 16 20
Cd4 Cd2 Ca1 63.19(7) 2 14_565
Cd9 Cd2 Ca1 66.55(3) . 14_565
Cd9 Cd2 Ca1 66.55(3) 16 14_565
Cd1 Cd2 Ca1 172.99(7) . 14_565
Cd3 Cd2 Ca1 64.93(6) . 14_565
Cd3 Cd2 Ca1 64.93(6) 16 14_565
Cd5 Cd2 Ca1 118.35(4) . 14_565
Cd5 Cd2 Ca1 118.35(4) 16 14_565
Cd2 Cd2 Ca1 114.30(7) 20 14_565
Cd4 Cd2 Ca2 67.92(5) 2 17
Cd9 Cd2 Ca2 126.01(5) . 17
Cd9 Cd2 Ca2 63.64(5) 16 17
Cd1 Cd2 Ca2 66.70(5) . 17
Cd3 Cd2 Ca2 172.69(5) . 17
Cd3 Cd2 Ca2 114.54(5) 16 17
Cd5 Cd2 Ca2 117.76(6) . 17
Cd5 Cd2 Ca2 62.47(4) 16 17
Cd2 Cd2 Ca2 114.04(4) 20 17
Ca1 Cd2 Ca2 118.69(7) 14_565 17
Cd4 Cd2 Ca2 67.92(5) 2 2
Cd9 Cd2 Ca2 63.64(5) . 2
Cd9 Cd2 Ca2 126.01(5) 16 2
Cd1 Cd2 Ca2 66.70(5) . 2
Cd3 Cd2 Ca2 114.54(5) . 2
Cd3 Cd2 Ca2 172.69(5) 16 2
Cd5 Cd2 Ca2 62.47(4) . 2
Cd5 Cd2 Ca2 117.76(6) 16 2
Cd2 Cd2 Ca2 114.04(4) 20 2
Ca1 Cd2 Ca2 118.69(7) 14_565 2
Ca2 Cd2 Ca2 69.98(9) 17 2
Cd7 Cd3 Cd7 66.67(5) 6 5_565
Cd7 Cd3 Cd2 172.06(4) 6 .
Cd7 Cd3 Cd2 115.29(3) 5_565 .
Cd7 Cd3 Cd2 115.29(3) 6 20
Cd7 Cd3 Cd2 172.06(4) 5_565 20
Cd2 Cd3 Cd2 61.65(4) . 20
Cd7 Cd3 Cd3 126.01(3) 6 16
Cd7 Cd3 Cd3 126.01(3) 5_565 16
Cd2 Cd3 Cd3 59.82(2) . 16
Cd2 Cd3 Cd3 59.82(2) 20 16
Cd7 Cd3 Cd9 118.31(4) 6 .
Cd7 Cd3 Cd9 64.09(3) 5_565 .
Cd2 Cd3 Cd9 58.80(2) . .
Cd2 Cd3 Cd9 109.37(4) 20 .
Cd3 Cd3 Cd9 112.41(2) 16 .
Cd7 Cd3 Cd9 64.09(3) 6 20
Cd7 Cd3 Cd9 118.31(4) 5_565 20
Cd2 Cd3 Cd9 109.37(4) . 20
Cd2 Cd3 Cd9 58.80(2) 20 20
Cd3 Cd3 Cd9 112.41(2) 16 20
Cd9 Cd3 Cd9 112.02(4) . 20
Cd7 Cd3 Cd8 76.84(3) 6 .
Cd7 Cd3 Cd8 76.84(3) 5_565 .
Cd2 Cd3 Cd8 111.04(3) . .
Cd2 Cd3 Cd8 111.04(3) 20 .
Cd3 Cd3 Cd8 60.542(18) 16 .
Cd9 Cd3 Cd8 122.93(2) . .
Cd9 Cd3 Cd8 122.93(2) 20 .
Cd7 Cd3 Cd5 113.02(4) 6 .
Cd7 Cd3 Cd5 113.02(4) 5_565 .
Cd2 Cd3 Cd5 59.04(3) . .
Cd2 Cd3 Cd5 59.04(3) 20 .
Cd3 Cd3 Cd5 107.37(2) 16 .
Cd9 Cd3 Cd5 59.73(2) . .
Cd9 Cd3 Cd5 59.73(2) 20 .
Cd8 Cd3 Cd5 167.91(4) . .
Cd7 Cd3 Ca3 64.23(6) 6 .
Cd7 Cd3 Ca3 64.23(6) 5_565 .
Cd2 Cd3 Ca3 109.15(6) . .
Cd2 Cd3 Ca3 109.15(6) 20 .
Cd3 Cd3 Ca3 166.63(7) 16 .
Cd9 Cd3 Ca3 62.26(3) . .
Cd9 Cd3 Ca3 62.26(3) 20 .
Cd8 Cd3 Ca3 132.82(7) . .
Cd5 Cd3 Ca3 59.26(7) . .
Cd7 Cd3 Ca1 123.81(5) 6 14_565
Cd7 Cd3 Ca1 67.70(2) 5_565 14_565
Cd2 Cd3 Ca1 62.74(4) . 14_565
Cd2 Cd3 Ca1 114.50(3) 20 14_565
Cd3 Cd3 Ca1 63.94(2) 16 14_565
Cd9 Cd3 Ca1 65.06(5) . 14_565
Cd9 Cd3 Ca1 172.10(5) 20 14_565
Cd8 Cd3 Ca1 62.29(5) . 14_565
Cd5 Cd3 Ca1 113.83(5) . 14_565
Ca3 Cd3 Ca1 119.57(4) . 14_565
Cd7 Cd3 Ca1 67.70(2) 6 15
Cd7 Cd3 Ca1 123.81(5) 5_565 15
Cd2 Cd3 Ca1 114.50(3) . 15
Cd2 Cd3 Ca1 62.74(4) 20 15
Cd3 Cd3 Ca1 63.94(2) 16 15
Cd9 Cd3 Ca1 172.10(5) . 15
Cd9 Cd3 Ca1 65.06(5) 20 15
Cd8 Cd3 Ca1 62.29(5) . 15
Cd5 Cd3 Ca1 113.83(5) . 15
Ca3 Cd3 Ca1 119.57(4) . 15
Ca1 Cd3 Ca1 116.78(9) 14_565 15
Cd2 Cd4 Cd2 114.98(6) 3 7
Cd2 Cd4 Cd12 108.772(13) 3 .
Cd2 Cd4 Cd12 108.772(13) 7 .
Cd2 Cd4 Cd12 108.772(13) 3 13_655
Cd2 Cd4 Cd12 108.772(13) 7 13_655
Cd12 Cd4 Cd12 106.44(6) . 13_655
Cd2 Cd4 Ca1 65.73(4) 3 13_655
Cd2 Cd4 Ca1 179.29(6) 7 13_655
Cd12 Cd4 Ca1 70.85(3) . 13_655
Cd12 Cd4 Ca1 70.85(3) 13_655 13_655
Cd2 Cd4 Ca1 179.29(6) 3 .
Cd2 Cd4 Ca1 65.73(4) 7 .
Cd12 Cd4 Ca1 70.85(3) . .
Cd12 Cd4 Ca1 70.85(3) 13_655 .
Ca1 Cd4 Ca1 113.57(9) 13_655 .
Cd2 Cd4 Cd9 56.040(16) 3 18
Cd2 Cd4 Cd9 117.07(3) 7 18
Cd12 Cd4 Cd9 133.88(4) . 18
Cd12 Cd4 Cd9 54.70(2) 13_655 18
Ca1 Cd4 Cd9 63.25(2) 13_655 18
Ca1 Cd4 Cd9 123.75(3) . 18
Cd2 Cd4 Cd9 117.07(3) 3 22
Cd2 Cd4 Cd9 56.040(16) 7 22
Cd12 Cd4 Cd9 54.70(2) . 22
Cd12 Cd4 Cd9 133.88(4) 13_655 22
Ca1 Cd4 Cd9 123.75(3) 13_655 22
Ca1 Cd4 Cd9 63.25(2) . 22
Cd9 Cd4 Cd9 168.95(6) 18 22
Cd2 Cd4 Cd9 56.040(16) 3 3
Cd2 Cd4 Cd9 117.07(3) 7 3
Cd12 Cd4 Cd9 54.70(2) . 3
Cd12 Cd4 Cd9 133.88(4) 13_655 3
Ca1 Cd4 Cd9 63.25(2) 13_655 3
Ca1 Cd4 Cd9 123.75(3) . 3
Cd9 Cd4 Cd9 105.01(3) 18 3
Cd9 Cd4 Cd9 73.89(3) 22 3
Cd2 Cd4 Cd9 117.07(3) 3 7
Cd2 Cd4 Cd9 56.040(16) 7 7
Cd12 Cd4 Cd9 133.88(4) . 7
Cd12 Cd4 Cd9 54.70(2) 13_655 7
Ca1 Cd4 Cd9 123.75(3) 13_655 7
Ca1 Cd4 Cd9 63.25(2) . 7
Cd9 Cd4 Cd9 73.89(3) 18 7
Cd9 Cd4 Cd9 105.01(3) 22 7
Cd9 Cd4 Cd9 168.95(6) 3 7
Cd2 Cd4 Ca2 63.41(3) 3 16
Cd2 Cd4 Ca2 63.41(3) 7 16
Cd12 Cd4 Ca2 160.38(6) . 16
Cd12 Cd4 Ca2 93.18(5) 13_655 16
Ca1 Cd4 Ca2 117.15(4) 13_655 16
Ca1 Cd4 Ca2 117.15(4) . 16
Cd9 Cd4 Ca2 58.72(4) 18 16
Cd9 Cd4 Ca2 111.03(5) 22 16
Cd9 Cd4 Ca2 111.03(5) 3 16
Cd9 Cd4 Ca2 58.72(4) 7 16
Cd2 Cd4 Ca2 63.41(3) 3 .
Cd2 Cd4 Ca2 63.41(3) 7 .
Cd12 Cd4 Ca2 93.18(5) . .
Cd12 Cd4 Ca2 160.38(6) 13_655 .
Ca1 Cd4 Ca2 117.15(4) 13_655 .
Ca1 Cd4 Ca2 117.15(4) . .
Cd9 Cd4 Ca2 111.03(5) 18 .
Cd9 Cd4 Ca2 58.72(4) 22 .
Cd9 Cd4 Ca2 58.72(4) 3 .
Cd9 Cd4 Ca2 111.03(5) 7 .
Ca2 Cd4 Ca2 67.20(10) 16 .
Cd1 Cd5 Cd13 121.09(4) . 20
Cd1 Cd5 Cd13 121.09(4) . .
Cd13 Cd5 Cd13 60.75(5) 20 .
Cd1 Cd5 Cd2 59.59(3) . .
Cd13 Cd5 Cd2 179.30(4) 20 .
Cd13 Cd5 Cd2 118.90(3) . .
Cd1 Cd5 Cd2 59.59(3) . 20
Cd13 Cd5 Cd2 118.90(3) 20 20
Cd13 Cd5 Cd2 179.30(5) . 20
Cd2 Cd5 Cd2 61.44(4) . 20
Cd1 Cd5 Cd9 112.28(3) . 20
Cd13 Cd5 Cd9 71.60(4) 20 20
Cd13 Cd5 Cd9 120.96(4) . 20
Cd2 Cd5 Cd9 108.33(4) . 20
Cd2 Cd5 Cd9 58.38(2) 20 20
Cd1 Cd5 Cd9 112.28(3) . .
Cd13 Cd5 Cd9 120.96(4) 20 .
Cd13 Cd5 Cd9 71.60(4) . .
Cd2 Cd5 Cd9 58.38(2) . .
Cd2 Cd5 Cd9 108.33(4) 20 .
Cd9 Cd5 Cd9 110.35(4) 20 .
Cd1 Cd5 Cd3 106.82(4) . .
Cd13 Cd5 Cd3 120.81(5) 20 .
Cd13 Cd5 Cd3 120.81(5) . .
Cd2 Cd5 Cd3 58.75(3) . .
Cd2 Cd5 Cd3 58.75(3) 20 .
Cd9 Cd5 Cd3 58.77(2) 20 .
Cd9 Cd5 Cd3 58.77(2) . .
Cd1 Cd5 Cd14 57.32(4) . .
Cd13 Cd5 Cd14 72.37(4) 20 .
Cd13 Cd5 Cd14 72.37(4) . .
Cd2 Cd5 Cd14 108.16(4) . .
Cd2 Cd5 Cd14 108.16(4) 20 .
Cd9 Cd5 Cd14 124.34(2) 20 .
Cd9 Cd5 Cd14 124.34(2) . .
Cd3 Cd5 Cd14 164.14(5) . .
Cd1 Cd5 Ca3 172.13(7) . .
Cd13 Cd5 Ca3 65.36(6) 20 .
Cd13 Cd5 Ca3 65.36(6) . .
Cd2 Cd5 Ca3 113.97(6) . .
Cd2 Cd5 Ca3 113.97(6) 20 .
Cd9 Cd5 Ca3 64.28(3) 20 .
Cd9 Cd5 Ca3 64.28(3) . .
Cd3 Cd5 Ca3 65.31(6) . .
Cd14 Cd5 Ca3 130.55(7) . .
Cd1 Cd5 Ca2 67.83(5) . 2
Cd13 Cd5 Ca2 115.19(7) 20 2
Cd13 Cd5 Ca2 62.72(5) . 2
Cd2 Cd5 Ca2 64.84(5) . 2
Cd2 Cd5 Ca2 117.90(6) 20 2
Cd9 Cd5 Ca2 172.40(6) 20 2
Cd9 Cd5 Ca2 63.65(5) . 2
Cd3 Cd5 Ca2 113.69(5) . 2
Cd14 Cd5 Ca2 62.54(5) . 2
Ca3 Cd5 Ca2 114.57(5) . 2
Cd1 Cd5 Ca2 67.83(5) . 6
Cd13 Cd5 Ca2 62.72(5) 20 6
Cd13 Cd5 Ca2 115.19(6) . 6
Cd2 Cd5 Ca2 117.90(6) . 6
Cd2 Cd5 Ca2 64.84(5) 20 6
Cd9 Cd5 Ca2 63.65(5) 20 6
Cd9 Cd5 Ca2 172.40(6) . 6
Cd3 Cd5 Ca2 113.69(5) . 6
Cd14 Cd5 Ca2 62.54(5) . 6
Ca3 Cd5 Ca2 114.57(5) . 6
Ca2 Cd5 Ca2 121.88(10) 2 6
Cd1 Cd6 Cd1 120.74(6) 14 3
Cd1 Cd6 Cd6 179.63(3) 14 14
Cd1 Cd6 Cd6 59.63(3) 3 14
Cd1 Cd6 Cd16 119.63(3) 14 .
Cd1 Cd6 Cd16 119.63(3) 3 .
Cd6 Cd6 Cd16 60.0 14 .
Cd1 Cd6 Cd6 59.63(3) 14 15
Cd1 Cd6 Cd6 179.63(3) 3 15
Cd6 Cd6 Cd6 120.0 14 15
Cd16 Cd6 Cd6 60.0 . 15
Cd1 Cd6 Cd17 118.22(4) 14 13
Cd1 Cd6 Cd17 118.22(4) 3 13
Cd6 Cd6 Cd17 61.43(3) 14 13
Cd16 Cd6 Cd17 17.0(2) . 13
Cd6 Cd6 Cd17 61.43(3) 15 13
Cd1 Cd6 Cd17 118.22(4) 14 .
Cd1 Cd6 Cd17 118.22(4) 3 .
Cd6 Cd6 Cd17 61.43(3) 14 .
Cd16 Cd6 Cd17 17.0(2) . .
Cd6 Cd6 Cd17 61.43(3) 15 .
Cd17 Cd6 Cd17 33.9(4) 13 .
Cd1 Cd6 Cd14 59.80(3) 14 5
Cd1 Cd6 Cd14 118.50(3) 3 5
Cd6 Cd6 Cd14 120.09(3) 14 5
Cd16 Cd6 Cd14 91.51(4) . 5
Cd6 Cd6 Cd14 61.63(2) 15 5
Cd17 Cd6 Cd14 105.43(17) 13 5
Cd17 Cd6 Cd14 77.54(17) . 5
Cd1 Cd6 Cd14 118.50(3) 14 18
Cd1 Cd6 Cd14 59.80(3) 3 18
Cd6 Cd6 Cd14 61.63(2) 14 18
Cd16 Cd6 Cd14 91.51(4) . 18
Cd6 Cd6 Cd14 120.09(3) 15 18
Cd17 Cd6 Cd14 77.54(17) 13 18
Cd17 Cd6 Cd14 105.43(17) . 18
Cd14 Cd6 Cd14 176.99(8) 5 18
Cd1 Cd6 Cd14 59.80(3) 14 14
Cd1 Cd6 Cd14 118.50(3) 3 14
Cd6 Cd6 Cd14 120.09(3) 14 14
Cd16 Cd6 Cd14 91.51(4) . 14
Cd6 Cd6 Cd14 61.63(2) 15 14
Cd17 Cd6 Cd14 77.54(17) 13 14
Cd17 Cd6 Cd14 105.43(17) . 14
Cd14 Cd6 Cd14 111.28(4) 5 14
Cd14 Cd6 Cd14 68.64(4) 18 14
Cd1 Cd6 Cd14 118.50(3) 14 3
Cd1 Cd6 Cd14 59.80(3) 3 3
Cd6 Cd6 Cd14 61.63(2) 14 3
Cd16 Cd6 Cd14 91.51(4) . 3
Cd6 Cd6 Cd14 120.09(3) 15 3
Cd17 Cd6 Cd14 105.43(17) 13 3
Cd17 Cd6 Cd14 77.54(17) . 3
Cd14 Cd6 Cd14 68.64(4) 5 3
Cd14 Cd6 Cd14 111.28(4) 18 3
Cd14 Cd6 Cd14 176.99(8) 14 3
Cd1 Cd6 Ca2 65.66(3) 14 .
Cd1 Cd6 Ca2 65.66(3) 3 .
Cd6 Cd6 Ca2 114.638(15) 14 .
Cd16 Cd6 Ca2 146.49(5) . .
Cd6 Cd6 Ca2 114.638(15) 15 .
Cd17 Cd6 Ca2 163.5(2) 13 .
Cd17 Cd6 Ca2 129.5(2) . .
Cd14 Cd6 Ca2 61.46(5) 5 .
Cd14 Cd6 Ca2 115.71(6) 18 .
Cd14 Cd6 Ca2 115.71(6) 14 .
Cd14 Cd6 Ca2 61.46(5) 3 .
Cd11 Cd7 Cd3 118.31(3) . 6_655
Cd11 Cd7 Cd3 118.31(3) . 5
Cd3 Cd7 Cd3 104.16(5) 6_655 5
Cd11 Cd7 Cd9 60.23(3) . 22
Cd3 Cd7 Cd9 123.62(4) 6_655 22
Cd3 Cd7 Cd9 59.33(2) 5 22
Cd11 Cd7 Cd9 60.23(3) . 6_655
Cd3 Cd7 Cd9 59.33(2) 6_655 6_655
Cd3 Cd7 Cd9 123.62(4) 5 6_655
Cd9 Cd7 Cd9 84.80(4) 22 6_655
Cd11 Cd7 Cd7 56.44(3) . 16_556
Cd3 Cd7 Cd7 126.01(3) 6_655 16_556
Cd3 Cd7 Cd7 126.01(3) 5 16_556
Cd9 Cd7 Cd7 100.43(2) 22 16_556
Cd9 Cd7 Cd7 100.43(2) 6_655 16_556
Cd11 Cd7 Cd7 136.19(2) . 2_655
Cd3 Cd7 Cd7 56.67(2) 6_655 2_655
Cd3 Cd7 Cd7 103.85(2) 5 2_655
Cd9 Cd7 Cd7 163.17(2) 22 2_655
Cd9 Cd7 Cd7 106.431(19) 6_655 2_655
Cd7 Cd7 Cd7 90.0 16_556 2_655
Cd11 Cd7 Cd7 136.19(2) . 3_665
Cd3 Cd7 Cd7 103.85(2) 6_655 3_665
Cd3 Cd7 Cd7 56.67(2) 5 3_665
Cd9 Cd7 Cd7 106.431(19) 22 3_665
Cd9 Cd7 Cd7 163.17(2) 6_655 3_665
Cd7 Cd7 Cd7 90.0 16_556 3_665
Cd7 Cd7 Cd7 60.0 2_655 3_665
Cd11 Cd7 Ca3 76.72(3) . 14_556
Cd3 Cd7 Ca3 164.93(4) 6_655 14_556
Cd3 Cd7 Ca3 64.95(3) 5 14_556
Cd9 Cd7 Ca3 61.25(5) 22 14_556
Cd9 Cd7 Ca3 134.94(5) 6_655 14_556
Cd7 Cd7 Ca3 61.80(3) 16_556 14_556
Cd7 Cd7 Ca3 114.04(5) 2_655 14_556
Cd7 Cd7 Ca3 61.77(3) 3_665 14_556
Cd11 Cd7 Ca3 76.72(3) . 15_656
Cd3 Cd7 Ca3 64.95(3) 6_655 15_656
Cd3 Cd7 Ca3 164.93(4) 5 15_656
Cd9 Cd7 Ca3 134.94(5) 22 15_656
Cd9 Cd7 Ca3 61.25(5) 6_655 15_656
Cd7 Cd7 Ca3 61.80(3) 16_556 15_656
Cd7 Cd7 Ca3 61.77(3) 2_655 15_656
Cd7 Cd7 Ca3 114.04(5) 3_665 15_656
Ca3 Cd7 Ca3 123.39(7) 14_556 15_656
Cd11 Cd7 Ca1 98.42(7) . .
Cd3 Cd7 Ca1 62.86(4) 6_655 .
Cd3 Cd7 Ca1 62.86(4) 5 .
Cd9 Cd7 Ca1 62.09(4) 22 .
Cd9 Cd7 Ca1 62.09(4) 6_655 .
Cd7 Cd7 Ca1 154.86(6) 16_556 .
Cd7 Cd7 Ca1 111.58(5) 2_655 .
Cd7 Cd7 Ca1 111.58(5) 3_665 .
Ca3 Cd7 Ca1 116.36(5) 14_556 .
Ca3 Cd7 Ca1 116.36(5) 15_656 .
Cd3 Cd8 Cd3 58.92(4) 18_565 3_565
Cd3 Cd8 Cd3 97.89(2) 18_565 16
Cd3 Cd8 Cd3 128.384(10) 3_565 16
Cd3 Cd8 Cd3 128.384(10) 18_565 2_665
Cd3 Cd8 Cd3 97.89(2) 3_565 2_665
Cd3 Cd8 Cd3 128.384(10) 16 2_665
Cd3 Cd8 Cd3 128.384(10) 18_565 .
Cd3 Cd8 Cd3 97.89(2) 3_565 .
Cd3 Cd8 Cd3 58.92(4) 16 .
Cd3 Cd8 Cd3 97.89(2) 2_665 .
Cd3 Cd8 Cd3 97.89(2) 18_565 17_665
Cd3 Cd8 Cd3 128.384(10) 3_565 17_665
Cd3 Cd8 Cd3 97.89(2) 16 17_665
Cd3 Cd8 Cd3 58.92(4) 2_665 17_665
Cd3 Cd8 Cd3 128.384(10) . 17_665
Cd3 Cd8 Ca1 64.192(5) 18_565 14_565
Cd3 Cd8 Ca1 64.192(5) 3_565 14_565
Cd3 Cd8 Ca1 64.192(5) 16 14_565
Cd3 Cd8 Ca1 150.542(18) 2_665 14_565
Cd3 Cd8 Ca1 64.192(5) . 14_565
Cd3 Cd8 Ca1 150.542(18) 17_665 14_565
Cd3 Cd8 Ca1 64.192(5) 18_565 13_665
Cd3 Cd8 Ca1 64.192(5) 3_565 13_665
Cd3 Cd8 Ca1 150.542(18) 16 13_665
Cd3 Cd8 Ca1 64.192(5) 2_665 13_665
Cd3 Cd8 Ca1 150.542(18) . 13_665
Cd3 Cd8 Ca1 64.192(5) 17_665 13_665
Ca1 Cd8 Ca1 120.0 14_565 13_665
Cd3 Cd8 Ca1 150.542(18) 18_565 15
Cd3 Cd8 Ca1 150.542(18) 3_565 15
Cd3 Cd8 Ca1 64.192(5) 16 15
Cd3 Cd8 Ca1 64.192(5) 2_665 15
Cd3 Cd8 Ca1 64.192(5) . 15
Cd3 Cd8 Ca1 64.192(5) 17_665 15
Ca1 Cd8 Ca1 120.0 14_565 15
Ca1 Cd8 Ca1 120.0 13_665 15
Cd12 Cd9 Cd2 108.70(4) 2 .
Cd12 Cd9 Cd10 69.88(4) 2 2
Cd2 Cd9 Cd10 135.97(4) . 2
Cd12 Cd9 Cd3 130.10(4) 2 .
Cd2 Cd9 Cd3 60.26(3) . .
Cd10 Cd9 Cd3 153.90(3) 2 .
Cd12 Cd9 Cd5 159.91(3) 2 .
Cd2 Cd9 Cd5 60.11(3) . .
Cd10 Cd9 Cd5 105.66(4) 2 .
Cd3 Cd9 Cd5 61.50(3) . .
Cd12 Cd9 Cd11 61.11(4) 2 14_566
Cd2 Cd9 Cd11 159.87(3) . 14_566
Cd10 Cd9 Cd11 59.81(4) 2 14_566
Cd3 Cd9 Cd11 111.36(4) . 14_566
Cd5 Cd9 Cd11 134.76(4) . 14_566
Cd12 Cd9 Cd7 90.98(2) 2 5_565
Cd2 Cd9 Cd7 110.02(3) . 5_565
Cd10 Cd9 Cd7 113.98(4) 2 5_565
Cd3 Cd9 Cd7 56.58(3) . 5_565
Cd5 Cd9 Cd7 108.33(3) . 5_565
Cd11 Cd9 Cd7 55.87(4) 14_566 5_565
Cd12 Cd9 Ca3 136.87(5) 2 .
Cd2 Cd9 Ca3 112.30(3) . .
Cd10 Cd9 Ca3 89.13(4) 2 .
Cd3 Cd9 Ca3 64.81(4) . .
Cd5 Cd9 Ca3 60.61(6) . .
Cd11 Cd9 Ca3 75.77(5) 14_566 .
Cd7 Cd9 Ca3 63.00(7) 5_565 .
Cd12 Cd9 Cd4 56.86(4) 2 2
Cd2 Cd9 Cd4 53.81(3) . 2
Cd10 Cd9 Cd4 100.50(3) 2 2
Cd3 Cd9 Cd4 104.94(3) . 2
Cd5 Cd9 Cd4 106.59(4) . 2
Cd11 Cd9 Cd4 117.85(4) 14_566 2
Cd7 Cd9 Cd4 120.60(4) 5_565 2
Ca3 Cd9 Cd4 166.00(4) . 2
Cd12 Cd9 Ca2 97.96(4) 2 2
Cd2 Cd9 Ca2 64.93(5) . 2
Cd10 Cd9 Ca2 71.64(5) 2 2
Cd3 Cd9 Ca2 115.05(4) . 2
Cd5 Cd9 Ca2 62.55(4) . 2
Cd11 Cd9 Ca2 131.06(5) 14_566 2
Cd7 Cd9 Ca2 170.77(4) 5_565 2
Ca3 Cd9 Ca2 110.89(9) . 2
Cd4 Cd9 Ca2 63.54(5) 2 2
Cd12 Cd9 Ca1 68.99(6) 2 14_565
Cd2 Cd9 Ca1 62.41(3) . 14_565
Cd10 Cd9 Ca1 138.80(6) 2 14_565
Cd3 Cd9 Ca1 63.20(6) . 14_565
Cd5 Cd9 Ca1 113.74(5) . 14_565
Cd11 Cd9 Ca1 97.49(2) 14_566 14_565
Cd7 Cd9 Ca1 64.74(5) 5_565 14_565
Ca3 Cd9 Ca1 120.15(9) . 14_565
Cd4 Cd9 Ca1 57.63(6) 2 14_565
Ca2 Cd9 Ca1 116.43(6) 2 14_565
Cd12 Cd9 Cd13 122.27(4) 2 .
Cd2 Cd9 Cd13 104.73(3) . .
Cd10 Cd9 Cd13 53.46(4) 2 .
Cd3 Cd9 Cd13 107.20(3) . .
Cd5 Cd9 Cd13 52.87(3) . .
Cd11 Cd9 Cd13 95.21(3) 14_566 .
Cd7 Cd9 Cd13 119.49(3) 5_565 .
Ca3 Cd9 Cd13 58.42(7) . .
Cd4 Cd9 Cd13 119.92(4) 2 .
Ca2 Cd9 Cd13 57.11(5) 2 .
Ca1 Cd9 Cd13 166.31(4) 14_565 .
Cd13 Cd10 Cd13 66.08(7) 3 7_556
Cd13 Cd10 Cd9 115.91(4) 3 7_556
Cd13 Cd10 Cd9 72.51(3) 7_556 7_556
Cd13 Cd10 Cd9 72.51(3) 3 3
Cd13 Cd10 Cd9 115.91(4) 7_556 3
Cd9 Cd10 Cd9 170.67(7) 7_556 3
Cd13 Cd10 Cd9 115.91(4) 3 22
Cd13 Cd10 Cd9 72.51(3) 7_556 22
Cd9 Cd10 Cd9 94.14(3) 7_556 22
Cd9 Cd10 Cd9 85.10(3) 3 22
Cd13 Cd10 Cd9 72.51(3) 3 18_556
Cd13 Cd10 Cd9 115.91(4) 7_556 18_556
Cd9 Cd10 Cd9 85.10(3) 7_556 18_556
Cd9 Cd10 Cd9 94.14(3) 3 18_556
Cd9 Cd10 Cd9 170.67(7) 22 18_556
Cd13 Cd10 Cd11 175.09(5) 3 .
Cd13 Cd10 Cd11 109.01(4) 7_556 .
Cd9 Cd10 Cd11 61.31(3) 7_556 .
Cd9 Cd10 Cd11 110.59(5) 3 .
Cd9 Cd10 Cd11 61.31(3) 22 .
Cd9 Cd10 Cd11 110.59(5) 18_556 .
Cd13 Cd10 Cd11 109.01(4) 3 13_656
Cd13 Cd10 Cd11 175.09(5) 7_556 13_656
Cd9 Cd10 Cd11 110.59(5) 7_556 13_656
Cd9 Cd10 Cd11 61.31(3) 3 13_656
Cd9 Cd10 Cd11 110.59(5) 22 13_656
Cd9 Cd10 Cd11 61.31(3) 18_556 13_656
Cd11 Cd10 Cd11 75.90(6) . 13_656
Cd13 Cd10 Cd12 125.90(2) 3 13_656
Cd13 Cd10 Cd12 125.90(2) 7_556 13_656
Cd9 Cd10 Cd12 54.54(2) 7_556 13_656
Cd9 Cd10 Cd12 117.80(4) 3 13_656
Cd9 Cd10 Cd12 117.80(4) 22 13_656
Cd9 Cd10 Cd12 54.54(2) 18_556 13_656
Cd11 Cd10 Cd12 56.52(3) . 13_656
Cd11 Cd10 Cd12 56.52(3) 13_656 13_656
Cd13 Cd10 Cd12 125.90(2) 3 .
Cd13 Cd10 Cd12 125.90(2) 7_556 .
Cd9 Cd10 Cd12 117.80(4) 7_556 .
Cd9 Cd10 Cd12 54.54(2) 3 .
Cd9 Cd10 Cd12 54.54(2) 22 .
Cd9 Cd10 Cd12 117.80(4) 18_556 .
Cd11 Cd10 Cd12 56.52(3) . .
Cd11 Cd10 Cd12 56.52(3) 13_656 .
Cd12 Cd10 Cd12 91.22(5) 13_656 .
Cd13 Cd10 Ca2 57.61(4) 3 .
Cd13 Cd10 Ca2 57.61(4) 7_556 .
Cd9 Cd10 Ca2 127.96(4) 7_556 .
Cd9 Cd10 Ca2 59.26(3) 3 .
Cd9 Cd10 Ca2 59.26(3) 22 .
Cd9 Cd10 Ca2 127.96(4) 18_556 .
Cd11 Cd10 Ca2 120.26(3) . .
Cd11 Cd10 Ca2 120.26(3) 13_656 .
Cd12 Cd10 Ca2 175.34(6) 13_656 .
Cd12 Cd10 Ca2 84.11(5) . .
Cd13 Cd10 Ca2 57.61(4) 3 16_556
Cd13 Cd10 Ca2 57.61(4) 7_556 16_556
Cd9 Cd10 Ca2 59.26(3) 7_556 16_556
Cd9 Cd10 Ca2 127.96(4) 3 16_556
Cd9 Cd10 Ca2 127.96(4) 22 16_556
Cd9 Cd10 Ca2 59.26(3) 18_556 16_556
Cd11 Cd10 Ca2 120.26(3) . 16_556
Cd11 Cd10 Ca2 120.26(3) 13_656 16_556
Cd12 Cd10 Ca2 84.11(5) 13_656 16_556
Cd12 Cd10 Ca2 175.34(6) . 16_556
Ca2 Cd10 Ca2 100.55(10) . 16_556
Cd7 Cd11 Cd7 67.12(6) 16_556 .
Cd7 Cd11 Cd10 120.83(2) 16_556 .
Cd7 Cd11 Cd10 120.83(2) . .
Cd7 Cd11 Cd10 120.83(2) 16_556 13_656
Cd7 Cd11 Cd10 120.83(2) . 13_656
Cd10 Cd11 Cd10 104.10(6) . 13_656
Cd7 Cd11 Cd12 160.92(5) 16_556 .
Cd7 Cd11 Cd12 93.80(3) . .
Cd10 Cd11 Cd12 68.09(3) . .
Cd10 Cd11 Cd12 68.09(3) 13_656 .
Cd7 Cd11 Cd12 93.80(3) 16_556 13_656
Cd7 Cd11 Cd12 160.92(5) . 13_656
Cd10 Cd11 Cd12 68.09(3) . 13_656
Cd10 Cd11 Cd12 68.09(3) 13_656 13_656
Cd12 Cd11 Cd12 105.28(6) . 13_656
Cd7 Cd11 Cd9 63.90(3) 16_556 15_656
Cd7 Cd11 Cd9 110.49(5) . 15_656
Cd10 Cd11 Cd9 125.68(4) . 15_656
Cd10 Cd11 Cd9 58.87(2) 13_656 15_656
Cd12 Cd11 Cd9 126.91(4) . 15_656
Cd12 Cd11 Cd9 57.65(2) 13_656 15_656
Cd7 Cd11 Cd9 110.49(5) 16_556 22
Cd7 Cd11 Cd9 63.90(3) . 22
Cd10 Cd11 Cd9 58.87(2) . 22
Cd10 Cd11 Cd9 125.68(4) 13_656 22
Cd12 Cd11 Cd9 57.65(2) . 22
Cd12 Cd11 Cd9 126.91(4) 13_656 22
Cd9 Cd11 Cd9 173.82(7) 15_656 22
Cd7 Cd11 Cd9 63.90(3) 16_556 7_556
Cd7 Cd11 Cd9 110.49(5) . 7_556
Cd10 Cd11 Cd9 58.87(2) . 7_556
Cd10 Cd11 Cd9 125.68(4) 13_656 7_556
Cd12 Cd11 Cd9 126.91(4) . 7_556
Cd12 Cd11 Cd9 57.65(2) 13_656 7_556
Cd9 Cd11 Cd9 88.47(3) 15_656 7_556
Cd9 Cd11 Cd9 91.19(3) 22 7_556
Cd7 Cd11 Cd9 110.49(5) 16_556 6_655
Cd7 Cd11 Cd9 63.90(3) . 6_655
Cd10 Cd11 Cd9 125.68(4) . 6_655
Cd10 Cd11 Cd9 58.87(2) 13_656 6_655
Cd12 Cd11 Cd9 57.65(2) . 6_655
Cd12 Cd11 Cd9 126.91(4) 13_656 6_655
Cd9 Cd11 Cd9 91.19(3) 15_656 6_655
Cd9 Cd11 Cd9 88.47(3) 22 6_655
Cd9 Cd11 Cd9 173.82(7) 7_556 6_655
Cd7 Cd11 Ca3 57.28(5) 16_556 15_656
Cd7 Cd11 Ca3 57.28(5) . 15_656
Cd10 Cd11 Ca3 177.51(7) . 15_656
Cd10 Cd11 Ca3 78.39(6) 13_656 15_656
Cd12 Cd11 Ca3 113.18(3) . 15_656
Cd12 Cd11 Ca3 113.18(3) 13_656 15_656
Cd9 Cd11 Ca3 55.53(4) 15_656 15_656
Cd9 Cd11 Ca3 119.73(5) 22 15_656
Cd9 Cd11 Ca3 119.73(5) 7_556 15_656
Cd9 Cd11 Ca3 55.53(4) 6_655 15_656
Cd7 Cd11 Ca3 57.28(5) 16_556 14_556
Cd7 Cd11 Ca3 57.28(5) . 14_556
Cd10 Cd11 Ca3 78.39(6) . 14_556
Cd10 Cd11 Ca3 177.51(7) 13_656 14_556
Cd12 Cd11 Ca3 113.18(3) . 14_556
Cd12 Cd11 Ca3 113.18(3) 13_656 14_556
Cd9 Cd11 Ca3 119.73(5) 15_656 14_556
Cd9 Cd11 Ca3 55.53(4) 22 14_556
Cd9 Cd11 Ca3 55.53(4) 7_556 14_556
Cd9 Cd11 Ca3 119.73(5) 6_655 14_556
Ca3 Cd11 Ca3 99.12(12) 15_656 14_556
Cd9 Cd12 Cd9 170.55(6) 3 6_655
Cd9 Cd12 Cd9 86.45(3) 3 22
Cd9 Cd12 Cd9 92.77(3) 6_655 22
Cd9 Cd12 Cd9 92.77(3) 3 19_655
Cd9 Cd12 Cd9 86.45(3) 6_655 19_655
Cd9 Cd12 Cd9 170.55(6) 22 19_655
Cd9 Cd12 Cd4 68.44(3) 3 .
Cd9 Cd12 Cd4 119.96(4) 6_655 .
Cd9 Cd12 Cd4 68.44(3) 22 .
Cd9 Cd12 Cd4 119.96(4) 19_655 .
Cd9 Cd12 Cd4 119.96(4) 3 13_655
Cd9 Cd12 Cd4 68.44(3) 6_655 13_655
Cd9 Cd12 Cd4 119.96(4) 22 13_655
Cd9 Cd12 Cd4 68.44(3) 19_655 13_655
Cd4 Cd12 Cd4 73.56(6) . 13_655
Cd9 Cd12 Cd11 110.49(4) 3 .
Cd9 Cd12 Cd11 61.25(3) 6_655 .
Cd9 Cd12 Cd11 61.25(3) 22 .
Cd9 Cd12 Cd11 110.49(4) 19_655 .
Cd4 Cd12 Cd11 129.54(2) . .
Cd4 Cd12 Cd11 129.54(2) 13_655 .
Cd9 Cd12 Cd11 61.25(3) 3 13_656
Cd9 Cd12 Cd11 110.49(4) 6_655 13_656
Cd9 Cd12 Cd11 110.49(4) 22 13_656
Cd9 Cd12 Cd11 61.25(3) 19_655 13_656
Cd4 Cd12 Cd11 129.54(2) . 13_656
Cd4 Cd12 Cd11 129.54(2) 13_655 13_656
Cd11 Cd12 Cd11 74.72(6) . 13_656
Cd9 Cd12 Cd10 116.59(4) 3 13_656
Cd9 Cd12 Cd10 55.58(2) 6_655 13_656
Cd9 Cd12 Cd10 116.59(4) 22 13_656
Cd9 Cd12 Cd10 55.58(2) 19_655 13_656
Cd4 Cd12 Cd10 172.39(5) . 13_656
Cd4 Cd12 Cd10 98.83(3) 13_655 13_656
Cd11 Cd12 Cd10 55.39(3) . 13_656
Cd11 Cd12 Cd10 55.39(3) 13_656 13_656
Cd9 Cd12 Cd10 55.58(2) 3 .
Cd9 Cd12 Cd10 116.59(4) 6_655 .
Cd9 Cd12 Cd10 55.58(2) 22 .
Cd9 Cd12 Cd10 116.59(4) 19_655 .
Cd4 Cd12 Cd10 98.83(3) . .
Cd4 Cd12 Cd10 172.39(5) 13_655 .
Cd11 Cd12 Cd10 55.39(3) . .
Cd11 Cd12 Cd10 55.39(3) 13_656 .
Cd10 Cd12 Cd10 88.78(5) 13_656 .
Cd9 Cd12 Ca1 62.55(3) 3 13_655
Cd9 Cd12 Ca1 124.71(4) 6_655 13_655
Cd9 Cd12 Ca1 124.71(4) 22 13_655
Cd9 Cd12 Ca1 62.55(3) 19_655 13_655
Cd4 Cd12 Ca1 58.15(4) . 13_655
Cd4 Cd12 Ca1 58.15(4) 13_655 13_655
Cd11 Cd12 Ca1 168.57(6) . 13_655
Cd11 Cd12 Ca1 93.86(5) 13_656 13_655
Cd10 Cd12 Ca1 118.09(3) 13_656 13_655
Cd10 Cd12 Ca1 118.09(3) . 13_655
Cd9 Cd12 Ca1 124.71(4) 3 .
Cd9 Cd12 Ca1 62.55(3) 6_655 .
Cd9 Cd12 Ca1 62.55(3) 22 .
Cd9 Cd12 Ca1 124.71(4) 19_655 .
Cd4 Cd12 Ca1 58.15(4) . .
Cd4 Cd12 Ca1 58.15(4) 13_655 .
Cd11 Cd12 Ca1 93.86(5) . .
Cd11 Cd12 Ca1 168.57(6) 13_656 .
Cd10 Cd12 Ca1 118.09(3) 13_656 .
Cd10 Cd12 Ca1 118.09(3) . .
Ca1 Cd12 Ca1 97.57(9) 13_655 .
Cd5 Cd13 Cd5 109.28(5) 16_556 .
Cd5 Cd13 Cd10 108.85(4) 16_556 2
Cd5 Cd13 Cd10 108.85(4) . 2
Cd5 Cd13 Cd13 59.63(3) 16_556 20
Cd5 Cd13 Cd13 59.63(3) . 20
Cd10 Cd13 Cd13 153.04(3) 2 20
Cd5 Cd13 Cd15 107.61(5) 16_556 2
Cd5 Cd13 Cd15 107.61(5) . 2
Cd10 Cd13 Cd15 114.55(5) 2 2
Cd13 Cd13 Cd15 92.41(4) 20 2
Cd5 Cd13 Cd13 125.36(2) 16_556 9_556
Cd5 Cd13 Cd13 125.36(2) . 9_556
Cd10 Cd13 Cd13 56.96(3) 2 9_556
Cd13 Cd13 Cd13 150.0 20 9_556
Cd15 Cd13 Cd13 57.59(4) 2 9_556
Cd5 Cd13 Ca2 173.83(5) 16_556 2
Cd5 Cd13 Ca2 64.65(3) . 2
Cd10 Cd13 Ca2 73.20(5) 2 2
Cd13 Cd13 Ca2 115.89(4) 20 2
Cd15 Cd13 Ca2 76.15(5) 2 2
Cd13 Cd13 Ca2 60.74(3) 9_556 2
Cd5 Cd13 Ca2 64.65(3) 16_556 17_556
Cd5 Cd13 Ca2 173.83(5) . 17_556
Cd10 Cd13 Ca2 73.20(5) 2 17_556
Cd13 Cd13 Ca2 115.89(4) 20 17_556
Cd15 Cd13 Ca2 76.15(5) 2 17_556
Cd13 Cd13 Ca2 60.74(3) 9_556 17_556
Ca2 Cd13 Ca2 121.38(6) 2 17_556
Cd5 Cd13 Ca3 61.50(3) 16_556 .
Cd5 Cd13 Ca3 61.50(3) . .
Cd10 Cd13 Ca3 89.47(6) 2 .
Cd13 Cd13 Ca3 63.57(4) 20 .
Cd15 Cd13 Ca3 155.98(7) 2 .
Cd13 Cd13 Ca3 146.43(4) 9_556 .
Ca2 Cd13 Ca3 113.10(5) 2 .
Ca2 Cd13 Ca3 113.10(5) 17_556 .
Cd5 Cd13 Cd9 55.53(3) 16_556 16_556
Cd5 Cd13 Cd9 116.58(5) . 16_556
Cd10 Cd13 Cd9 54.03(3) 2 16_556
Cd13 Cd13 Cd9 106.76(2) 20 16_556
Cd15 Cd13 Cd9 135.71(3) 2 16_556
Cd13 Cd13 Cd9 96.58(2) 9_556 16_556
Ca2 Cd13 Cd9 125.23(7) 2 16_556
Ca2 Cd13 Cd9 59.56(5) 17_556 16_556
Ca3 Cd13 Cd9 58.39(4) . 16_556
Cd5 Cd13 Cd9 116.58(5) 16_556 .
Cd5 Cd13 Cd9 55.53(3) . .
Cd10 Cd13 Cd9 54.03(3) 2 .
Cd13 Cd13 Cd9 106.76(2) 20 .
Cd15 Cd13 Cd9 135.71(3) 2 .
Cd13 Cd13 Cd9 96.58(2) 9_556 .
Ca2 Cd13 Cd9 59.56(5) 2 .
Ca2 Cd13 Cd9 125.23(7) 17_556 .
Ca3 Cd13 Cd9 58.39(4) . .
Cd9 Cd13 Cd9 76.82(4) 16_556 .
Cd15 Cd14 Cd15 67.81(6) 15_556 2
Cd15 Cd14 Cd1 142.87(5) 15_556 .
Cd15 Cd14 Cd1 142.87(5) 2 .
Cd15 Cd14 Cd6 149.16(8) 15_556 2
Cd15 Cd14 Cd6 109.18(3) 2 2
Cd1 Cd14 Cd6 57.01(4) . 2
Cd15 Cd14 Cd6 109.18(3) 15_556 15
Cd15 Cd14 Cd6 149.16(8) 2 15
Cd1 Cd14 Cd6 57.01(4) . 15
Cd6 Cd14 Cd6 56.74(5) 2 15
Cd15 Cd14 Cd5 103.94(7) 15_556 .
Cd15 Cd14 Cd5 103.94(7) 2 .
Cd1 Cd14 Cd5 56.98(4) . .
Cd6 Cd14 Cd5 106.43(5) 2 .
Cd6 Cd14 Cd5 106.43(5) 15 .
Cd15 Cd14 Ca2 75.87(6) 15_556 6
Cd15 Cd14 Ca2 135.79(7) 2 6
Cd1 Cd14 Ca2 67.01(5) . 6
Cd6 Cd14 Ca2 114.91(6) 2 6
Cd6 Cd14 Ca2 66.59(5) 15 6
Cd5 Cd14 Ca2 60.97(4) . 6
Cd15 Cd14 Ca2 135.79(7) 15_556 2
Cd15 Cd14 Ca2 75.87(6) 2 2
Cd1 Cd14 Ca2 67.01(5) . 2
Cd6 Cd14 Ca2 66.59(5) 2 2
Cd6 Cd14 Ca2 114.91(6) 15 2
Cd5 Cd14 Ca2 60.97(4) . 2
Ca2 Cd14 Ca2 118.93(7) 6 2
Cd15 Cd14 Cd14 111.91(5) 15_556 6
Cd15 Cd14 Cd14 53.63(3) 2 6
Cd1 Cd14 Cd14 105.149(18) . 6
Cd6 Cd14 Cd14 55.681(18) 2 6
Cd6 Cd14 Cd14 105.02(4) 15 6
Cd5 Cd14 Cd14 119.989(1) . 6
Ca2 Cd14 Cd14 170.58(5) 6 6
Ca2 Cd14 Cd14 59.65(4) 2 6
Cd15 Cd14 Cd14 53.63(3) 15_556 5
Cd15 Cd14 Cd14 111.91(5) 2 5
Cd1 Cd14 Cd14 105.149(18) . 5
Cd6 Cd14 Cd14 105.02(3) 2 5
Cd6 Cd14 Cd14 55.681(18) 15 5
Cd5 Cd14 Cd14 119.989(1) . 5
Ca2 Cd14 Cd14 59.65(4) 6 5
Ca2 Cd14 Cd14 170.58(5) 2 5
Cd14 Cd14 Cd14 120.0 6 5
Cd15 Cd14 Ca4 74.9(3) 15_556 .
Cd15 Cd14 Ca4 74.9(3) 2 .
Cd1 Cd14 Ca4 124.4(4) . .
Cd6 Cd14 Ca4 74.8(4) 2 .
Cd6 Cd14 Ca4 74.8(4) 15 .
Cd5 Cd14 Ca4 178.6(4) . .
Ca2 Cd14 Ca4 119.26(8) 6 .
Ca2 Cd14 Ca4 119.26(8) 2 .
Cd14 Cd14 Ca4 60.042(13) 6 .
Cd14 Cd14 Ca4 60.042(12) 5 .
Cd14 Cd15 Cd14 169.86(12) 3 14_556
Cd14 Cd15 Cd14 72.75(5) 3 5
Cd14 Cd15 Cd14 106.31(4) 14_556 5
Cd14 Cd15 Cd14 106.31(4) 3 18_556
Cd14 Cd15 Cd14 72.75(5) 14_556 18_556
Cd14 Cd15 Cd14 169.86(12) 5 18_556
Cd14 Cd15 Cd13 113.11(6) 3 7_556
Cd14 Cd15 Cd13 75.92(5) 14_556 7_556
Cd14 Cd15 Cd13 75.92(5) 5 7_556
Cd14 Cd15 Cd13 113.11(6) 18_556 7_556
Cd14 Cd15 Cd13 75.92(5) 3 3
Cd14 Cd15 Cd13 113.11(6) 14_556 3
Cd14 Cd15 Cd13 113.11(6) 5 3
Cd14 Cd15 Cd13 75.92(5) 18_556 3
Cd13 Cd15 Cd13 64.82(7) 7_556 3
Cd14 Cd15 Cd15 56.09(3) 3 14_556
Cd14 Cd15 Cd15 118.00(5) 14_556 14_556
Cd14 Cd15 Cd15 118.00(5) 5 14_556
Cd14 Cd15 Cd15 56.09(3) 18_556 14_556
Cd13 Cd15 Cd15 152.41(4) 7_556 14_556
Cd13 Cd15 Cd15 87.59(4) 3 14_556
Cd14 Cd15 Cd15 118.00(5) 3 15_556
Cd14 Cd15 Cd15 56.09(3) 14_556 15_556
Cd14 Cd15 Cd15 56.09(3) 5 15_556
Cd14 Cd15 Cd15 118.00(5) 18_556 15_556
Cd13 Cd15 Cd15 87.59(4) 7_556 15_556
Cd13 Cd15 Cd15 152.41(4) 3 15_556
Cd15 Cd15 Cd15 120.0 14_556 15_556
Cd14 Cd15 Ca4 58.9(2) 3 .
Cd14 Cd15 Ca4 111.7(2) 14_556 .
Cd14 Cd15 Ca4 58.9(2) 5 .
Cd14 Cd15 Ca4 111.7(2) 18_556 .
Cd13 Cd15 Ca4 134.7(2) 7_556 .
Cd13 Cd15 Ca4 134.7(2) 3 .
Cd15 Cd15 Ca4 65.38(9) 14_556 .
Cd15 Cd15 Ca4 65.38(9) 15_556 .
Cd14 Cd15 Ca4 111.7(2) 3 13_556
Cd14 Cd15 Ca4 58.9(2) 14_556 13_556
Cd14 Cd15 Ca4 111.7(2) 5 13_556
Cd14 Cd15 Ca4 58.9(2) 18_556 13_556
Cd13 Cd15 Ca4 134.7(2) 7_556 13_556
Cd13 Cd15 Ca4 134.7(2) 3 13_556
Cd15 Cd15 Ca4 65.38(9) 14_556 13_556
Cd15 Cd15 Ca4 65.38(9) 15_556 13_556
Ca4 Cd15 Ca4 67.2(6) . 13_556
Cd14 Cd15 Ca2 130.58(7) 3 16_556
Cd14 Cd15 Ca2 57.92(4) 14_556 16_556
Cd14 Cd15 Ca2 130.58(7) 5 16_556
Cd14 Cd15 Ca2 57.92(4) 18_556 16_556
Cd13 Cd15 Ca2 55.29(5) 7_556 16_556
Cd13 Cd15 Ca2 55.29(5) 3 16_556
Cd15 Cd15 Ca2 109.71(2) 14_556 16_556
Cd15 Cd15 Ca2 109.71(2) 15_556 16_556
Ca4 Cd15 Ca2 166.0(3) . 16_556
Ca4 Cd15 Ca2 98.8(3) 13_556 16_556
Cd14 Cd15 Ca2 57.92(4) 3 .
Cd14 Cd15 Ca2 130.58(7) 14_556 .
Cd14 Cd15 Ca2 57.92(4) 5 .
Cd14 Cd15 Ca2 130.58(7) 18_556 .
Cd13 Cd15 Ca2 55.29(5) 7_556 .
Cd13 Cd15 Ca2 55.29(5) 3 .
Cd15 Cd15 Ca2 109.71(2) 14_556 .
Cd15 Cd15 Ca2 109.71(2) 15_556 .
Ca4 Cd15 Ca2 98.8(3) . .
Ca4 Cd15 Ca2 166.0(3) 13_556 .
Ca2 Cd15 Ca2 95.17(10) 16_556 .
Cd17 Cd16 Cd17 180.0 13 .
Cd17 Cd16 Ca4 0.0 13 13
Cd17 Cd16 Ca4 180.0 . 13
Cd17 Cd16 Ca4 180.0 13 .
Cd17 Cd16 Ca4 0.0 . .
Ca4 Cd16 Ca4 180.000(1) 13 .
Cd17 Cd16 Cd6 90.0 13 15
Cd17 Cd16 Cd6 90.0 . 15
Ca4 Cd16 Cd6 90.0 13 15
Ca4 Cd16 Cd6 90.0 . 15
Cd17 Cd16 Cd6 90.0 13 3
Cd17 Cd16 Cd6 90.0 . 3
Ca4 Cd16 Cd6 90.0 13 3
Ca4 Cd16 Cd6 90.0 . 3
Cd6 Cd16 Cd6 180.00(11) 15 3
Cd17 Cd16 Cd6 90.0 13 .
Cd17 Cd16 Cd6 90.0 . .
Ca4 Cd16 Cd6 90.0 13 .
Ca4 Cd16 Cd6 90.0 . .
Cd6 Cd16 Cd6 60.0 15 .
Cd6 Cd16 Cd6 120.0 3 .
Cd17 Cd16 Cd6 90.0 13 14
Cd17 Cd16 Cd6 90.0 . 14
Ca4 Cd16 Cd6 90.0 13 14
Ca4 Cd16 Cd6 90.0 . 14
Cd6 Cd16 Cd6 120.0 15 14
Cd6 Cd16 Cd6 60.0 3 14
Cd6 Cd16 Cd6 60.0 . 14
Cd17 Cd16 Cd6 90.0 13 2
Cd17 Cd16 Cd6 90.0 . 2
Ca4 Cd16 Cd6 90.0 13 2
Ca4 Cd16 Cd6 90.0 . 2
Cd6 Cd16 Cd6 60.0 15 2
Cd6 Cd16 Cd6 120.0 3 2
Cd6 Cd16 Cd6 120.0 . 2
Cd6 Cd16 Cd6 180.0 14 2
Cd17 Cd16 Cd6 90.0 13 13
Cd17 Cd16 Cd6 90.0 . 13
Ca4 Cd16 Cd6 90.0 13 13
Ca4 Cd16 Cd6 90.0 . 13
Cd6 Cd16 Cd6 120.0 15 13
Cd6 Cd16 Cd6 60.0 3 13
Cd6 Cd16 Cd6 180.0 . 13
Cd6 Cd16 Cd6 120.0 14 13
Cd6 Cd16 Cd6 60.0 2 13
Cd16 Cd17 Cd17 0.0 . 13
Cd16 Cd17 Ca4 180.000(1) . .
Cd17 Cd17 Ca4 180.000(1) 13 .
Cd16 Cd17 Cd6 73.0(2) . 3
Cd17 Cd17 Cd6 73.0(2) 13 3
Ca4 Cd17 Cd6 107.0(2) . 3
Cd16 Cd17 Cd6 73.0(2) . 15
Cd17 Cd17 Cd6 73.0(2) 13 15
Ca4 Cd17 Cd6 107.0(2) . 15
Cd6 Cd17 Cd6 146.1(4) 3 15
Cd16 Cd17 Cd6 73.0(2) . 14
Cd17 Cd17 Cd6 73.0(2) 13 14
Ca4 Cd17 Cd6 107.0(2) . 14
Cd6 Cd17 Cd6 57.14(7) 3 14
Cd6 Cd17 Cd6 111.85(18) 15 14
Cd16 Cd17 Cd6 73.0(2) . .
Cd17 Cd17 Cd6 73.0(2) 13 .
Ca4 Cd17 Cd6 107.0(2) . .
Cd6 Cd17 Cd6 111.85(18) 3 .
Cd6 Cd17 Cd6 57.14(7) 15 .
Cd6 Cd17 Cd6 57.14(7) 14 .
Cd16 Cd17 Cd6 73.0(2) . 2
Cd17 Cd17 Cd6 73.0(2) 13 2
Ca4 Cd17 Cd6 107.0(2) . 2
Cd6 Cd17 Cd6 111.85(18) 3 2
Cd6 Cd17 Cd6 57.14(7) 15 2
Cd6 Cd17 Cd6 146.1(4) 14 2
Cd6 Cd17 Cd6 111.85(18) . 2
Cd16 Cd17 Cd6 73.0(2) . 13
Cd17 Cd17 Cd6 73.0(2) 13 13
Ca4 Cd17 Cd6 107.0(2) . 13
Cd6 Cd17 Cd6 57.14(7) 3 13
Cd6 Cd17 Cd6 111.85(18) 15 13
Cd6 Cd17 Cd6 111.85(18) 14 13
Cd6 Cd17 Cd6 146.1(4) . 13
Cd6 Cd17 Cd6 57.14(7) 2 13
Cd16 Cd17 Ca4 0.000(1) . 13
Cd17 Cd17 Ca4 0.0 13 13
Ca4 Cd17 Ca4 180.000(1) . 13
Cd6 Cd17 Ca4 73.0(2) 3 13
Cd6 Cd17 Ca4 73.0(2) 15 13
Cd6 Cd17 Ca4 73.0(2) 14 13
Cd6 Cd17 Ca4 73.0(2) . 13
Cd6 Cd17 Ca4 73.0(2) 2 13
Cd6 Cd17 Ca4 73.0(2) 13 13
Cd4 Ca1 Cd4 66.43(9) 13_655 .
Cd4 Ca1 Cd2 51.09(4) 13_655 15_655
Cd4 Ca1 Cd2 117.52(11) . 15_655
Cd4 Ca1 Cd2 117.52(11) 13_655 7
Cd4 Ca1 Cd2 51.09(4) . 7
Cd2 Ca1 Cd2 168.60(13) 15_655 7
Cd4 Ca1 Cd8 146.78(4) 13_655 13_665
Cd4 Ca1 Cd8 146.78(4) . 13_665
Cd2 Ca1 Cd8 95.70(7) 15_655 13_665
Cd2 Ca1 Cd8 95.70(7) 7 13_665
Cd4 Ca1 Cd3 97.38(3) 13_655 6_655
Cd4 Ca1 Cd3 150.04(6) . 6_655
Cd2 Ca1 Cd3 52.33(3) 15_655 6_655
Cd2 Ca1 Cd3 136.82(8) 7 6_655
Cd8 Ca1 Cd3 53.52(5) 13_665 6_655
Cd4 Ca1 Cd3 97.38(3) 13_655 15_655
Cd4 Ca1 Cd3 150.04(6) . 15_655
Cd2 Ca1 Cd3 52.33(3) 15_655 15_655
Cd2 Ca1 Cd3 136.82(8) 7 15_655
Cd8 Ca1 Cd3 53.52(5) 13_665 15_655
Cd3 Ca1 Cd3 52.11(5) 6_655 15_655
Cd4 Ca1 Cd3 150.04(6) 13_655 5
Cd4 Ca1 Cd3 97.38(3) . 5
Cd2 Ca1 Cd3 136.82(8) 15_655 5
Cd2 Ca1 Cd3 52.33(3) 7 5
Cd8 Ca1 Cd3 53.52(5) 13_665 5
Cd3 Ca1 Cd3 84.67(8) 6_655 5
Cd3 Ca1 Cd3 107.04(11) 15_655 5
Cd4 Ca1 Cd3 150.04(6) 13_655 14
Cd4 Ca1 Cd3 97.38(3) . 14
Cd2 Ca1 Cd3 136.82(8) 15_655 14
Cd2 Ca1 Cd3 52.33(3) 7 14
Cd8 Ca1 Cd3 53.52(5) 13_665 14
Cd3 Ca1 Cd3 107.04(11) 6_655 14
Cd3 Ca1 Cd3 84.67(8) 15_655 14
Cd3 Ca1 Cd3 52.11(5) 5 14
Cd4 Ca1 Cd9 59.12(4) 13_655 6_655
Cd4 Ca1 Cd9 98.96(8) . 6_655
Cd2 Ca1 Cd9 51.033(17) 15_655 6_655
Cd2 Ca1 Cd9 125.90(4) 7 6_655
Cd8 Ca1 Cd9 102.34(6) 13_665 6_655
Cd3 Ca1 Cd9 51.74(2) 6_655 6_655
Cd3 Ca1 Cd9 92.90(3) 15_655 6_655
Cd3 Ca1 Cd9 101.73(4) 5 6_655
Cd3 Ca1 Cd9 150.84(9) 14 6_655
Cd4 Ca1 Cd9 59.12(4) 13_655 15_655
Cd4 Ca1 Cd9 98.96(8) . 15_655
Cd2 Ca1 Cd9 51.033(17) 15_655 15_655
Cd2 Ca1 Cd9 125.90(4) 7 15_655
Cd8 Ca1 Cd9 102.34(6) 13_665 15_655
Cd3 Ca1 Cd9 92.90(3) 6_655 15_655
Cd3 Ca1 Cd9 51.74(2) 15_655 15_655
Cd3 Ca1 Cd9 150.84(9) 5 15_655
Cd3 Ca1 Cd9 101.73(4) 14 15_655
Cd9 Ca1 Cd9 99.37(4) 6_655 15_655
Cd4 Ca1 Cd9 98.96(8) 13_655 7
Cd4 Ca1 Cd9 59.12(4) . 7
Cd2 Ca1 Cd9 125.90(4) 15_655 7
Cd2 Ca1 Cd9 51.033(17) 7 7
Cd8 Ca1 Cd9 102.34(6) 13_665 7
Cd3 Ca1 Cd9 150.84(10) 6_655 7
Cd3 Ca1 Cd9 101.73(4) 15_655 7
Cd3 Ca1 Cd9 92.90(3) 5 7
Cd3 Ca1 Cd9 51.74(2) 14 7
Cd9 Ca1 Cd9 155.33(13) 6_655 7
Cd9 Ca1 Cd9 75.28(3) 15_655 7
Cd13 Ca2 Cd13 58.52(6) 7_556 3
Cd13 Ca2 Cd5 52.63(3) 7_556 5
Cd13 Ca2 Cd5 111.12(8) 3 5
Cd13 Ca2 Cd5 111.12(8) 7_556 3
Cd13 Ca2 Cd5 52.63(3) 3 3
Cd5 Ca2 Cd5 163.38(10) 5 3
Cd13 Ca2 Cd9 63.33(5) 7_556 22
Cd13 Ca2 Cd9 97.61(8) 3 22
Cd5 Ca2 Cd9 53.80(3) 5 22
Cd5 Ca2 Cd9 125.90(8) 3 22
Cd13 Ca2 Cd9 97.61(8) 7_556 3
Cd13 Ca2 Cd9 63.33(5) 3 3
Cd5 Ca2 Cd9 125.90(8) 5 3
Cd5 Ca2 Cd9 53.80(3) 3 3
Cd9 Ca2 Cd9 72.99(6) 22 3
Cd13 Ca2 Cd14 94.70(8) 7_556 3
Cd13 Ca2 Cd14 65.67(6) 3 3
Cd5 Ca2 Cd14 116.61(8) 5 3
Cd5 Ca2 Cd14 56.49(4) 3 3
Cd9 Ca2 Cd14 157.77(10) 22 3
Cd9 Ca2 Cd14 108.94(4) 3 3
Cd13 Ca2 Cd14 65.67(6) 7_556 5
Cd13 Ca2 Cd14 94.70(8) 3 5
Cd5 Ca2 Cd14 56.49(4) 5 5
Cd5 Ca2 Cd14 116.61(8) 3 5
Cd9 Ca2 Cd14 108.94(4) 22 5
Cd9 Ca2 Cd14 157.77(10) 3 5
Cd14 Ca2 Cd14 60.71(7) 3 5
Cd13 Ca2 Cd2 149.01(9) 7_556 3
Cd13 Ca2 Cd2 99.49(4) 3 3
Cd5 Ca2 Cd2 142.70(9) 5 3
Cd5 Ca2 Cd2 52.69(3) 3 3
Cd9 Ca2 Cd2 102.65(8) 22 3
Cd9 Ca2 Cd2 51.43(3) 3 3
Cd14 Ca2 Cd2 94.85(4) 3 3
Cd14 Ca2 Cd2 143.16(9) 5 3
Cd13 Ca2 Cd2 99.49(4) 7_556 7
Cd13 Ca2 Cd2 149.01(9) 3 7
Cd5 Ca2 Cd2 52.69(3) 5 7
Cd5 Ca2 Cd2 142.70(9) 3 7
Cd9 Ca2 Cd2 51.43(3) 22 7
Cd9 Ca2 Cd2 102.65(8) 3 7
Cd14 Ca2 Cd2 143.16(9) 3 7
Cd14 Ca2 Cd2 94.85(4) 5 7
Cd2 Ca2 Cd2 90.18(7) 3 7
Cd13 Ca2 Cd1 97.36(4) 7_556 14
Cd13 Ca2 Cd1 144.92(9) 3 14
Cd5 Ca2 Cd1 50.54(3) 5 14
Cd5 Ca2 Cd1 139.61(9) 3 14
Cd9 Ca2 Cd1 92.01(3) 22 14
Cd9 Ca2 Cd1 151.03(9) 3 14
Cd14 Ca2 Cd1 94.36(8) 3 14
Cd14 Ca2 Cd1 50.39(4) 5 14
Cd2 Ca2 Cd1 111.20(8) 3 14
Cd2 Ca2 Cd1 50.32(4) 7 14
Cd13 Ca2 Cd1 144.92(9) 7_556 3
Cd13 Ca2 Cd1 97.36(4) 3 3
Cd5 Ca2 Cd1 139.61(9) 5 3
Cd5 Ca2 Cd1 50.54(3) 3 3
Cd9 Ca2 Cd1 151.03(9) 22 3
Cd9 Ca2 Cd1 92.01(3) 3 3
Cd14 Ca2 Cd1 50.39(4) 3 3
Cd14 Ca2 Cd1 94.36(8) 5 3
Cd2 Ca2 Cd1 50.32(4) 3 3
Cd2 Ca2 Cd1 111.20(8) 7 3
Cd1 Ca2 Cd1 89.83(7) 14 3
Cd5 Ca3 Cd5 95.88(12) . 16_556
Cd5 Ca3 Cd9 55.11(3) . .
Cd5 Ca3 Cd9 113.25(9) 16_556 .
Cd5 Ca3 Cd9 113.25(9) . 11_556
Cd5 Ca3 Cd9 55.11(3) 16_556 11_556
Cd9 Ca3 Cd9 164.79(14) . 11_556
Cd5 Ca3 Cd9 113.25(9) . 16_556
Cd5 Ca3 Cd9 55.11(3) 16_556 16_556
Cd9 Ca3 Cd9 81.24(3) . 16_556
Cd9 Ca3 Cd9 96.74(3) 11_556 16_556
Cd5 Ca3 Cd9 55.11(3) . 20
Cd5 Ca3 Cd9 113.25(9) 16_556 20
Cd9 Ca3 Cd9 96.74(4) . 20
Cd9 Ca3 Cd9 81.24(3) 11_556 20
Cd9 Ca3 Cd9 164.79(14) 16_556 20
Cd5 Ca3 Cd13 53.14(6) . .
Cd5 Ca3 Cd13 53.14(6) 16_556 .
Cd9 Ca3 Cd13 63.18(5) . .
Cd9 Ca3 Cd13 102.37(9) 11_556 .
Cd9 Ca3 Cd13 63.18(5) 16_556 .
Cd9 Ca3 Cd13 102.37(9) 20 .
Cd5 Ca3 Cd13 53.14(6) . 20
Cd5 Ca3 Cd13 53.14(6) 16_556 20
Cd9 Ca3 Cd13 102.37(9) . 20
Cd9 Ca3 Cd13 63.18(5) 11_556 20
Cd9 Ca3 Cd13 102.37(9) 16_556 20
Cd9 Ca3 Cd13 63.18(5) 20 20
Cd13 Ca3 Cd13 52.86(8) . 20
Cd5 Ca3 Cd7 148.10(3) . 15_556
Cd5 Ca3 Cd7 98.47(3) 16_556 15_556
Cd9 Ca3 Cd7 139.43(12) . 15_556
Cd9 Ca3 Cd7 55.75(3) 11_556 15_556
Cd9 Ca3 Cd7 98.29(6) 16_556 15_556
Cd9 Ca3 Cd7 93.01(5) 20 15_556
Cd13 Ca3 Cd7 151.21(5) . 15_556
Cd13 Ca3 Cd7 117.09(3) 20 15_556
Cd5 Ca3 Cd7 98.47(3) . 6
Cd5 Ca3 Cd7 148.10(3) 16_556 6
Cd9 Ca3 Cd7 98.29(6) . 6
Cd9 Ca3 Cd7 93.01(5) 11_556 6
Cd9 Ca3 Cd7 139.43(12) 16_556 6
Cd9 Ca3 Cd7 55.75(3) 20 6
Cd13 Ca3 Cd7 151.21(5) . 6
Cd13 Ca3 Cd7 117.09(3) 20 6
Cd7 Ca3 Cd7 56.41(6) 15_556 6
Cd5 Ca3 Cd7 148.10(3) . 14_566
Cd5 Ca3 Cd7 98.47(3) 16_556 14_566
Cd9 Ca3 Cd7 93.01(5) . 14_566
Cd9 Ca3 Cd7 98.29(6) 11_556 14_566
Cd9 Ca3 Cd7 55.75(3) 16_556 14_566
Cd9 Ca3 Cd7 139.43(12) 20 14_566
Cd13 Ca3 Cd7 117.09(3) . 14_566
Cd13 Ca3 Cd7 151.21(5) 20 14_566
Cd7 Ca3 Cd7 56.46(7) 15_556 14_566
Cd7 Ca3 Cd7 83.93(10) 6 14_566
Cd5 Ca3 Cd7 98.47(3) . 5_565
Cd5 Ca3 Cd7 148.10(3) 16_556 5_565
Cd9 Ca3 Cd7 55.75(3) . 5_565
Cd9 Ca3 Cd7 139.43(12) 11_556 5_565
Cd9 Ca3 Cd7 93.01(5) 16_556 5_565
Cd9 Ca3 Cd7 98.29(6) 20 5_565
Cd13 Ca3 Cd7 117.09(3) . 5_565
Cd13 Ca3 Cd7 151.21(5) 20 5_565
Cd7 Ca3 Cd7 83.93(10) 15_556 5_565
Cd7 Ca3 Cd7 56.46(7) 6 5_565
Cd7 Ca3 Cd7 56.41(6) 14_566 5_565
Cd17 Ca4 Cd16 0.0 . .
Cd17 Ca4 Cd14 87.1(4) . 4
Cd16 Ca4 Cd14 87.1(4) . 4
Cd17 Ca4 Cd14 87.1(4) . .
Cd16 Ca4 Cd14 87.1(4) . .
Cd14 Ca4 Cd14 174.2(8) 4 .
Cd17 Ca4 Cd14 87.1(4) . 6
Cd16 Ca4 Cd14 87.1(4) . 6
Cd14 Ca4 Cd14 119.75(7) 4 6
Cd14 Ca4 Cd14 59.92(2) . 6
Cd17 Ca4 Cd14 87.1(4) . 2
Cd16 Ca4 Cd14 87.1(4) . 2
Cd14 Ca4 Cd14 59.92(2) 4 2
Cd14 Ca4 Cd14 119.75(7) . 2
Cd14 Ca4 Cd14 59.92(2) 6 2
Cd17 Ca4 Cd14 87.1(4) . 5
Cd16 Ca4 Cd14 87.1(4) . 5
Cd14 Ca4 Cd14 119.75(7) 4 5
Cd14 Ca4 Cd14 59.92(2) . 5
Cd14 Ca4 Cd14 119.75(7) 6 5
Cd14 Ca4 Cd14 174.2(8) 2 5
Cd17 Ca4 Cd14 87.1(4) . 3
Cd16 Ca4 Cd14 87.1(4) . 3
Cd14 Ca4 Cd14 59.92(2) 4 3
Cd14 Ca4 Cd14 119.75(7) . 3
Cd14 Ca4 Cd14 174.2(8) 6 3
Cd14 Ca4 Cd14 119.75(7) 2 3
Cd14 Ca4 Cd14 59.92(2) 5 3
Cd17 Ca4 Cd17 0.000(1) . 13
Cd16 Ca4 Cd17 0.0 . 13
Cd14 Ca4 Cd17 87.1(4) 4 13
Cd14 Ca4 Cd17 87.1(4) . 13
Cd14 Ca4 Cd17 87.1(4) 6 13
Cd14 Ca4 Cd17 87.1(4) 2 13
Cd14 Ca4 Cd17 87.1(4) 5 13
Cd14 Ca4 Cd17 87.1(4) 3 13
Cd17 Ca4 Cd15 123.6(3) . 15_556
Cd16 Ca4 Cd15 123.6(3) . 15_556
Cd14 Ca4 Cd15 138.4(5) 4 15_556
Cd14 Ca4 Cd15 46.15(12) . 15_556
Cd14 Ca4 Cd15 91.6(2) 6 15_556
Cd14 Ca4 Cd15 138.4(5) 2 15_556
Cd14 Ca4 Cd15 46.15(12) 5 15_556
Cd14 Ca4 Cd15 91.6(2) 3 15_556
Cd17 Ca4 Cd15 123.6(3) 13 15_556
Cd17 Ca4 Cd15 123.6(3) . 2
Cd16 Ca4 Cd15 123.6(3) . 2
Cd14 Ca4 Cd15 138.4(5) 4 2
Cd14 Ca4 Cd15 46.15(12) . 2
Cd14 Ca4 Cd15 46.15(12) 6 2
Cd14 Ca4 Cd15 91.6(2) 2 2
Cd14 Ca4 Cd15 91.6(2) 5 2
Cd14 Ca4 Cd15 138.4(5) 3 2
Cd17 Ca4 Cd15 123.6(3) 13 2
Cd15 Ca4 Cd15 49.24(18) 15_556 2
Cd17 Ca4 Cd15 123.6(3) . .
Cd16 Ca4 Cd15 123.6(3) . .
Cd14 Ca4 Cd15 91.6(2) 4 .
Cd14 Ca4 Cd15 91.6(2) . .
Cd14 Ca4 Cd15 138.4(5) 6 .
Cd14 Ca4 Cd15 138.4(5) 2 .
Cd14 Ca4 Cd15 46.15(12) 5 .
Cd14 Ca4 Cd15 46.15(12) 3 .
Cd17 Ca4 Cd15 123.6(3) 13 .
Cd15 Ca4 Cd15 49.24(18) 15_556 .
Cd15 Ca4 Cd15 92.4(4) 2 .
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
Cd1 Cd6 2.7872(14) 15
Cd1 Cd6 2.7872(14) 2
Cd1 Cd5 2.8609(12) .
Cd1 Cd5 2.8609(12) 16
Cd1 Cd14 2.8720(15) 16
Cd1 Cd14 2.8720(15) .
Cd1 Cd2 2.8756(15) 20
Cd1 Cd2 2.8756(15) .
Cd1 Ca2 3.432(2) 6
Cd1 Ca2 3.432(2) 15
Cd1 Ca2 3.432(2) 17
Cd1 Ca2 3.432(2) 2
Cd2 Cd4 2.7953(12) 2
Cd2 Cd9 2.8729(9) .
Cd2 Cd9 2.8729(9) 16
Cd2 Cd3 2.9161(11) .
Cd2 Cd3 2.9161(11) 16
Cd2 Cd5 2.9248(10) .
Cd2 Cd5 2.9248(10) 16
Cd2 Cd2 2.9884(18) 20
Cd2 Ca1 3.2749(11) 14_565
Cd2 Ca2 3.328(2) 17
Cd2 Ca2 3.328(2) 2
Cd3 Cd7 2.8491(10) 6
Cd3 Cd7 2.8491(10) 5_565
Cd3 Cd2 2.9161(11) 20
Cd3 Cd3 2.9315(19) 16
Cd3 Cd9 2.9357(9) .
Cd3 Cd9 2.9357(9) 20
Cd3 Cd8 2.9805(10) .
Cd3 Cd5 3.0173(14) .
Cd3 Ca3 3.3294(15) .
Cd3 Ca1 3.337(2) 14_565
Cd3 Ca1 3.337(2) 15
Cd4 Cd2 2.7953(12) 3
Cd4 Cd2 2.7953(12) 7
Cd4 Cd12 2.9334(15) .
Cd4 Cd12 2.9334(15) 13_655
Cd4 Ca1 3.206(3) 13_655
Cd4 Ca1 3.206(3) .
Cd4 Cd9 3.2580(9) 18
Cd4 Cd9 3.2580(9) 22
Cd4 Cd9 3.2580(9) 3
Cd4 Cd9 3.2580(9) 7
Cd4 Ca2 3.449(3) 16
Cd4 Ca2 3.449(3) .
Cd5 Cd13 2.8674(11) 20
Cd5 Cd13 2.8674(11) .
Cd5 Cd2 2.9248(10) 20
Cd5 Cd9 2.9651(10) 20
Cd5 Cd9 2.9651(10) .
Cd5 Cd14 3.110(2) .
Cd5 Ca3 3.150(3) .
Cd5 Ca2 3.2608(8) 2
Cd5 Ca2 3.2608(8) 6
Cd6 Cd1 2.7872(14) 14
Cd6 Cd1 2.7872(14) 3
Cd6 Cd6 2.8185(16) 14
Cd6 Cd16 2.8185(16) .
Cd6 Cd6 2.8185(16) 15
Cd6 Cd17 2.947(3) 13
Cd6 Cd17 2.947(3) .
Cd6 Cd14 2.9660(13) 5
Cd6 Cd14 2.9660(13) 18
Cd6 Cd14 2.9660(13) 14
Cd6 Cd14 2.9660(13) 3
Cd6 Ca2 3.457(3) .
Cd7 Cd11 2.8297(17) .
Cd7 Cd3 2.8491(10) 6_655
Cd7 Cd3 2.8491(10) 5
Cd7 Cd9 3.0701(12) 22
Cd7 Cd9 3.0701(12) 6_655
Cd7 Cd7 3.128(2) 16_556
Cd7 Cd7 3.1312(19) 2_655
Cd7 Cd7 3.1312(19) 3_665
Cd7 Ca3 3.310(3) 14_556
Cd7 Ca3 3.310(3) 15_656
Cd7 Ca1 3.469(2) .
Cd8 Cd3 2.9805(10) 18_565
Cd8 Cd3 2.9805(10) 3_565
Cd8 Cd3 2.9805(10) 16
Cd8 Cd3 2.9805(10) 2_665
Cd8 Cd3 2.9805(10) 17_665
Cd8 Ca1 3.282(4) 14_565
Cd8 Ca1 3.282(4) 13_665
Cd8 Ca1 3.282(4) 15
Cd9 Cd12 2.8593(8) 2
Cd9 Cd10 2.8957(8) 2
Cd9 Cd11 2.9675(8) 14_566
Cd9 Cd7 3.0701(12) 5_565
Cd9 Ca3 3.2565(10) .
Cd9 Cd4 3.2580(9) 2
Cd9 Ca2 3.293(2) 2
Cd9 Ca1 3.3900(12) 14_565
Cd9 Cd13 3.4125(16) .
Cd10 Cd13 2.875(2) 3
Cd10 Cd13 2.875(2) 7_556
Cd10 Cd9 2.8957(8) 7_556
Cd10 Cd9 2.8957(8) 3
Cd10 Cd9 2.8957(8) 22
Cd10 Cd9 2.8957(8) 18_556
Cd10 Cd11 2.9240(17) .
Cd10 Cd11 2.9240(17) 13_656
Cd10 Cd12 3.2962(16) 13_656
Cd10 Cd12 3.2962(16) .
Cd10 Ca2 3.636(3) .
Cd10 Ca2 3.636(3) 16_556
Cd11 Cd7 2.8297(17) 16_556
Cd11 Cd10 2.9240(17) 13_656
Cd11 Cd12 2.9635(15) .
Cd11 Cd12 2.9634(15) 13_656
Cd11 Cd9 2.9675(8) 15_656
Cd11 Cd9 2.9675(8) 22
Cd11 Cd9 2.9675(8) 7_556
Cd11 Cd9 2.9675(8) 6_655
Cd11 Ca3 3.8287(18) 15_656
Cd11 Ca3 3.8287(18) 14_556
Cd12 Cd9 2.8593(8) 3
Cd12 Cd9 2.8593(8) 6_655
Cd12 Cd9 2.8593(8) 22
Cd12 Cd9 2.8593(8) 19_655
Cd12 Cd4 2.9334(15) 13_655
Cd12 Cd11 2.9634(15) 13_656
Cd12 Cd10 3.2962(16) 13_656
Cd12 Ca1 3.566(3) 13_655
Cd12 Ca1 3.566(3) .
Cd13 Cd5 2.8674(11) 16_556
Cd13 Cd10 2.875(2) 2
Cd13 Cd13 2.900(3) 20
Cd13 Cd15 2.924(3) 2
Cd13 Cd13 3.135(2) 9_556
Cd13 Ca2 3.207(3) 2
Cd13 Ca2 3.207(3) 17_556
Cd13 Ca3 3.258(4) .
Cd13 Cd9 3.4125(16) 16_556
Cd14 Cd15 2.8197(11) 15_556
Cd14 Cd15 2.8197(11) 2
Cd14 Cd6 2.9660(13) 2
Cd14 Cd6 2.9660(13) 15
Cd14 Ca2 3.309(3) 6
Cd14 Ca2 3.309(3) 2
Cd14 Cd14 3.3445(18) 6
Cd14 Cd14 3.3445(18) 5
Cd14 Ca4 3.349(2) .
Cd15 Cd14 2.8197(11) 3
Cd15 Cd14 2.8197(11) 14_556
Cd15 Cd14 2.8197(11) 5
Cd15 Cd14 2.8197(11) 18_556
Cd15 Cd13 2.924(3) 7_556
Cd15 Cd13 2.924(3) 3
Cd15 Cd15 3.146(2) 14_556
Cd15 Cd15 3.146(2) 15_556
Cd15 Ca4 3.776(13) .
Cd15 Ca4 3.776(13) 13_556
Cd15 Ca2 3.788(3) 16_556
Cd15 Ca2 3.788(3) .
Cd16 Cd17 0.860(11) 13
Cd16 Cd17 0.860(11) .
Cd16 Ca4 2.62(2) 13
Cd16 Ca4 2.62(2) .
Cd16 Cd6 2.8185(16) 15
Cd16 Cd6 2.8185(16) 3
Cd16 Cd6 2.8185(16) 14
Cd16 Cd6 2.8185(16) 2
Cd16 Cd6 2.8185(16) 13
Cd17 Cd17 1.72(2) 13
Cd17 Ca4 1.76(3) .
Cd17 Cd6 2.947(3) 3
Cd17 Cd6 2.947(3) 15
Cd17 Cd6 2.947(3) 14
Cd17 Cd6 2.947(3) 2
Cd17 Cd6 2.947(3) 13
Cd17 Ca4 3.48(3) 13
Ca1 Cd4 3.206(3) 13_655
Ca1 Cd2 3.2749(11) 15_655
Ca1 Cd2 3.2749(11) 7
Ca1 Cd8 3.282(4) 13_665
Ca1 Cd3 3.337(2) 6_655
Ca1 Cd3 3.337(2) 15_655
Ca1 Cd3 3.337(2) 5
Ca1 Cd3 3.337(2) 14
Ca1 Cd9 3.3900(12) 6_655
Ca1 Cd9 3.3900(12) 15_655
Ca1 Cd9 3.3900(12) 7
Ca2 Cd13 3.207(3) 7_556
Ca2 Cd13 3.207(3) 3
Ca2 Cd5 3.2608(8) 5
Ca2 Cd5 3.2608(8) 3
Ca2 Cd9 3.293(2) 22
Ca2 Cd9 3.293(2) 3
Ca2 Cd14 3.309(3) 3
Ca2 Cd14 3.309(3) 5
Ca2 Cd2 3.328(2) 3
Ca2 Cd2 3.328(2) 7
Ca2 Cd1 3.432(2) 14
Ca2 Cd1 3.432(2) 3
Ca3 Cd5 3.150(3) 16_556
Ca3 Cd9 3.2565(10) 11_556
Ca3 Cd9 3.2565(10) 16_556
Ca3 Cd9 3.2565(10) 20
Ca3 Cd13 3.258(4) 20
Ca3 Cd7 3.310(3) 15_556
Ca3 Cd7 3.310(3) 6
Ca3 Cd7 3.310(3) 14_566
Ca3 Cd7 3.310(3) 5_565
Ca4 Cd14 3.349(2) 4
Ca4 Cd14 3.349(2) 6
Ca4 Cd14 3.349(2) 2
Ca4 Cd14 3.349(2) 5
Ca4 Cd14 3.349(2) 3
Ca4 Cd17 3.48(3) 13
Ca4 Cd15 3.776(13) 15_556
Ca4 Cd15 3.776(13) 2
